Sometimes the tensile stressed construction ma-terials fail brittly also at much lower stress than it corresponds to the tensile strength determined at the smooth test piece. This instable brittle fracture conduced to very rapid and unexpected fracture and therefore it is very dangerous. It goes out from cracks or other defects which eﬀect the stress concentration which is present in real machine parts at any time. At the design of constructions resistant to the brittle failure the so-called transition access is often used. It secures that the transition temperature is enough under the temperature range when the machine part will be used (HERTZBERG 1989; KETTUNEN, KUOK-KALA 2003).

One of the most used tests of the transition
tem-perature determination is the Charpy impact test
(ČSN EN 10 045-1) when the test specimen with
the notch is impact stressed by means of the
pen-dulum edge (SIH 1973, 1978). The tests are carried
out in the suﬃcient temperature range and the
rela-tion between the measured impact energy values
(*KV* – J) and the temperature (*T* – °C) is called the
transition curve. Its behaviour using the materials
of the b.c.c lattice shows the well-known “S”
char-acter. The transition curve can be divided into three
signiﬁcant ranges:

1. the low temperature range where the brittle failure occurs – the impact energy values are low, 2. the transition range – the signiﬁcant increase of

the impact energy values and as a rule with the high spread of measured values (caused by the diﬀerent failure mode),

3. the higher temperature range where the ductile failure occurs – the impact energy values are high.

The typical property of transition curves is the high spread of the measured impact energy values, above all in the transition range, which is for us the most important, but in the higher temperature range, too. However the values do not fall under a deﬁnite limit and the failures are always ductile. The representa-tion of measured values using the continuous curve demands a suitable method of smoothing. Except the nonparametric methods of smoothing (splains – excel etc.) the possibility of regression exists using the suitable regression functions which contain the regression parameters. Their values together with the regression function type describe unambigu-ously the transition curve (OWEN, FAWKES 1983; SIH 1968; HERÁK, CHOTĚBORSKÝ 2004).

Most often the transition curve is described as the hyperbolic tangent function in the form

**Mathematical function for the transition curves **

**description**

**R. CHOTĚBORSKÝ**

**1**

_{, D. HERÁK}

_{, D. HERÁK}

**2**

_{, V. BEZOUŠKA}

_{, V. BEZOUŠKA}

**3**

_{,}

_{,}

_{P. HRABĚ}

_{P. HRABĚ}

**1**

_{, M. MÜLLER}

_{, M. MÜLLER}

**1**

1

_{Department of Material and Engineering Technologies, Technical Faculty, }

_{Department of Material and Engineering Technologies, Technical Faculty, }

*Czech University of Agriculture in Prague, Prague, Czech Republic*

2

_{Department of Mechanics and Engineering, Technical Faculty, Czech University }

_{Department of Mechanics and Engineering, Technical Faculty, Czech University }

*of Agriculture in Prague, Prague, Czech Republic*

3

_{Department of Electrotechnical Engineering and Automation, Technical Faculty, }

_{Department of Electrotechnical Engineering and Automation, Technical Faculty, }

*Czech University of Agriculture in Prague, Prague, Czech Republic*

**ABSTRACT**: Toughness is one of important material properties. At present steel is still the most used material. Owing
to the temperature this material can fail both brittly and ductily. Therefore we look for the temperature above which the
material will failur ductily. The Charpy impact test is one of methods how to determine the ductility by the temperature
– transition access in the determined temperature range. The measured data ﬁle is large and it requires the interlay by
a curve which presents the relation between the impact energy and the temperature.

*KV* = ƒ(*T*) = *a* + *b* × tgh [*c* × (*T* – *d*)] (1)

where: *T* – the temperature,

*a, b, c, d* – the parameters as the results of the

regres-sion calculations,

*a *– the mean of the upper and lower levels of the
transition curve,

*b* – a half of upper and lower level diﬀerence,
*c* – the slope of the transition curve in the transition

range,

*d* – the suitable chosen parameter.

It presents the temperature of the curve asymme-try midpoint. It can be identiﬁed with the transition temperature as the curve inﬂexion point.

Then the expression (1) is possible to written:
*L* + *H* *H* – *L* 2 × (*T* – *T _{tr}*)

*KV* = + × tgh (2)
2 2 ∆*T*

This equation contents already the clear and simple parameters:

*H *– the upper impact energy level,
*L* – the lower impact energy level,
*T _{tr}* – the transition temperature,

*∆T*– the transition range width.

The further function of the comparable curve from is the arcustangent function (3)

*L* + *H* *H* – *L* π × (*T* – *T _{tr}*)

*KV* = + × arctg (3)
2 π ∆*T*

These functions are in possession of a deﬁnite limiting. It is the possibility of the curvature choice in the transition curve bending (Fig. 1).

The curvature can be simply changed – using the
powers of the initial function tgh(*x*) and arctg(*x*)
when the exponent determinates the curvature
bending.

*L* + *H* *H* – *L*

*KV* = + × sgn (*T* – *Ttr*) ×

2 2

2 × |*T* – *Ttr*|

1

×

## [

tgh## (

## )

*n*

## ]

*n*(4) ∆

*T*

where the signum function is deﬁned by the
rela-tions sgn *(x) = –*1 for *x* < 0, sgn (0) = 0, sgn (*x*) = 1
for *x* > 0.

In the equation (4) three variables can be changed for the suitable description:

*T _{tr}* – the inﬂex point position,
∆

*T*– the transition range width,

*n*– the exponent.

In this case the exponent determines the bend
sharpness of the curve bending. The sharp bend is in
the case if *n < *1. If *n > *1 the curve bending is milder
as is shown in Fig. 2.

In some cases the measured values *KV* cannot
be interlined using the above presented transition
curves function. In this case the function with the
oﬀ-centre position of the inﬂexion point is possible
to use, namely the function of the type exp(*x*).

*H* – *L* 1 + *p*

*KV* = *L* + × exp

## [

× (*T*–

*Ttr*)

## ]

for*T < Ttr*

1 + *p * ∆*T*
*H* – *L* 1 + *p*

*KV* = *H* – × exp

## [

– × (*T*–

*T*)

_{tr}## ]

1 +*p p*× ∆

*T*

for *T > T _{tr}* (5)

where: *p* – the suitable selected parameter.

In the case of the equation (5) we look for the
„*p*“ parameter, the inﬂexion point position and the
transition range width. Seeing that the equation of
the transition curve description is composed from
two parts, in this case it is possible to look for two
parameters „*p*“ particularly for each part, when the
upper and the lower bend must be described by
dif-ferent way. Fig. 3 shows the function (5) course for
diﬀerent parameters „*p _{L}*“ and „

*p*“, where „

_{H}*p*“ aﬀects

_{L}Fig. 1. Course of the hyperbolic tangent (*KV*_{tgh(t)}) and

arcus-tangent (*KV*_{arctg(t)}) Fig. 2. Signum function for various exponents

Im pa ct e ne rg y (J ) Temperature (°C) 100 80 60 40 20 0

–100 –50 0 50 100

*n* = 1
*n* = 0.1
*n* = 5

Im pa ct e ne rg y (J ) Temperature (°C)

–100 –50 0 50 100

the curve bending under the inﬂexion point, „*pH*“

over the inﬂexion point.

**MATERIAL AND METHODS**

The steel 21MnTiB with a feritic-pearlitic struc-ture (Fig. 4) and with the chemical composition (see Table 1) was used as the material for the experimen-tal description of the transition curve. This steel was cold formed using the broaching of the wire. The amount of the deformation was 10%. From this semi-product the specimens with V-notch (ČSN EN 10 045-1) for the Charpy impact test were made. The specimens were temperature treated in the bath of ethanol cooled using the liquid nitrogen on test tem-perature. Then the specimens were broken using the Charpy impact machine and the impact energy was read. The measured values are presented in Table 2. This values used for transition curve description.

For the transition curve description the function (2), (3), (4), (5) were selected. The function param-eters were calculated in MathLab.

**Algorithm notation in MathLab**

For compiling of the algorithm in MathLab the
arithmetic means of the impact energy measured
values of single sets of measuring are necessary.
This arithmetic mean values were used as “entry of
impact energy values”. For upper and lower limits of
the curve the arithmetic mean of the impact energy
value at the lowest “*L*” or highest “H” test
tempera-ture was used. The transition curve equation must
be in such a form and such coeﬃcients must be used,
when the MathLab software operate. The parameter
“*C*” is the arithmetic mean of the highest and the
lowest impact energy. The parameter “*D*” is a half of

Im

pa

ct

e

ne

rg

y

(J

)

Temperature (°C) 100

80

60

40

20

–100 –50 0 50 100

*p _{L}* = 1,

*p*1

_{H }=*p*= 0.2,

_{L}*p*5

_{H }=*p*= 5,

_{L}*p*0.15

_{H }=Fig. 3. Function (5) with the oﬀ-centre position of the inﬂexion
point for various parameters „*p*“

Table 1. Chemical composition of the steel 21MnTiB (weight percentage)

C Mn Si B Cu Ti Al P

0.2 0.89 0.09 0.005 0.057 0.015 0.03 0.015

Table 2. Measured values of the impact energy

Test temperature (°C) Impact energy value (J)

–75 10, 25, 15, 20

–60 36, 30, 20, 25

–50 50, 30, 40, 25

–40 70, 50, 40, 60

–20 70, 90, 80, 100

0 110, 90, 100, 70

20 95, 110, 90, 80

10 µ

Fig. 4. Ferritic-pearlitic structure, ﬁne-grained laminated to transition pearlitic

Fig. 5. Graphic representation of the measured values

Im

pa

ct

e

ne

rg

y

(J

)

Temperature (°C) 120

100

80

60

40

20

0

L = 18%h – the lowest impact energy value

H = 94%h – the highest impact energy value

% deviations calculation

C = (L + H)/2 – calculation of the parameter „C“

D = (H – L)/2 – calculation of the parameter „D“

T = (–75 –60 –50 –40 –20 0 20) – entry of the temperatures

Y = (18 28 36 55 85 93 94) – entry of the impact energy values

a =–50 – estimation of the parameter „a“ (transition temperature)

b = 0 – estimation of the parameter „b“ (transition range width)

consA = a; %Ttr – inﬂexion point of the curve

consB = b; %delta t – transition range width

for j = 1:700 – number of loops for the parameter „b“ calculation

b = b + 0.1 – step value for the parameter „b“ calculation

a = –50

for i = 1:700 – number of loops for the parameter „a“ calculation

a = a + 0.1 – step value for the parameter „a“ calculation

for k = 1:7

Kv(k) = C +D × tanh(2 × (T(k)-a)/b) – the curve equation

end

odch(i,j) = ((Y(1) – Kv(1))^2 +(Y(2) – Kv(2))^2 +(Y(3) – Kv(3))^2 +(Y(4) – Kv(4))^2 +(Y(5) – Kv(5))^2 +(Y(6) – Kv(6))^2 +(Y(7) – Kv(7))^2)

end end

%determing of min minim1 = min;

minim2 = min(minim1);

%determining of the minimum ordinates for j = 1:700

for i = 1:700

if odch(i,j)==minim2 pozA = i;

pozB = j; end; end end

%coeﬃcients calculation

b = pozB × 0.1 + consB – value of the sought parameter „b“

a = pozA × 0.1 + consA – value of the sought parameter „a“

%graph drawing

tep = –80:1:20 – entry of the range and axis step

vyst = C +D × tanh(2 × (tep – a)/b); plot(tep,vyst)

axis(–90 30 10 100) – adjustment for the axis range representation

hold on plot(T,Y,’r+’)

the highest and the lowest impact energy diﬀerence.

**RESULTS**

From the calculation of looking for the unknown parameters of the equation we get the unambiguous description curve, where mere by a introducing of

*KV* = 27 J value it is possible to get the transition
tem-perature using the method of the minimum energy. For
the further method of looking for the transition curve
equation namely using the method of the curve
inﬂex-ion point, the transitinﬂex-ion temperature value is one if the
demanded parameters already at the calculation.

When we look for another function than the hyper-bolic tangent type used by us in Mathlab, which de-scribes better the relation between the impact energy and the temperature, we can use the functions (3), (4), (5). These functions can be suitably chosen for the curve description or the algorithm can be modiﬁed by looking for such functions parameters, which have the minimal deviations from the measured values.

Fig. 7 presents the functions (2), (3), (4), (5), which
describe the measured values of the impact energy.
For these functions the same values of the upper (*H*)
and lower (*L*) limits were entered in the same way as
for the model program. At the arcustangent function
(3) the same parameters were looked for as at the
function (2). But the arcustangent function demands
to look not only for the inﬂexion point and the
transi-tion range width, but in additransi-tion to look for the limits

*H* and *L*. The signum function has the same curve as
the hyperbolic tangent function and is unambiguous
for the description. The exponential function (5) is of
the deﬁcient curvature in the curve bendings.

**CONCLUSIONS**

The interlay of the impact energy values using the function which unambiguously describes the

transition curve is one of possibilities. By a simple entry of energy limits we get the transition tem-peratures, which are the guide for the construction design.

The suitable chosen function for the transition curve description or for the entry in the algorithm of a suitable function from many offered gives the possibility to define the measured values evalua-tion with more precision. In our opinion the values entry in MathLab program and the curve plotting inclusive the transfer in the text editors is more simply and the results are more accurate than when using the accessible tabulator processor excel. In addition the searched results can be automated, as the transition temperature determination using the minimum energy method, which is used for the making of the constructional steels truncated sym-bols, or if need be, for the transition temperature as the inflexion point searching. In MathLab cal-culation the inflexion point of demanded param-eters.

The transition curves and transition temperatures determination is one of the most used tests. In this paper we attempted to outline the possibilities for the more eﬀective and accurate transition curves determination and for required the data. The model presented in this paper is possible to be used for the hyperbolic tangent function parameters determina-tion. For the other functions the notation must be modiﬁed in the appurtenant form.

**References**

HERÁK D., CHOTĚBORSKÝ R., 2004. The mathematical descriptions transitions curve. In: 9. medzinárodné sym-pózium jakost a spolehlivost. Nitra, SPU: 89–92.

Fig. 6. Course of the hyperbolic tangent function after the measured values approximation

Fig. 7. Functions (2) – tgh(*t*), (3) – arctg(*t*), (4) – sgn(*t*),
(5) – expd(*q*), and exph(*z*) describe the measured impact
ener-gy values. B_{m,l} are the impact energy arithmetic means

Im

pa

ct

e

ne

rg

y

(J

)

Temperature (°C) 100

80

60

40

20

0

–80 –60 –40 –20 0 20

Temperature (°C) 120

100

80

60

40

20

0

–80 –70 –60 –50 –40 –30 –20 –10 0 10 20 30

Im

pa

ct

e

ne

rg

y

(J

)

B_{m,1}
+ +
tgh(*t*)

arctg(*t*)

sgn(*t*)

expd(*q*)

HERTZBERG R.W., 1989. Deformation and Fracture Mechan-ics of Engineering Materials. New York, Wiley: 680. KETTUNEN O., KUOKKALA V., 2003. Plastic Deformation

and Strain Hardening. Trans Tech Publications. Zurich, Uetikon: 410.

KUNCICKY D., 2004. MatLab Programming. Upper Saddle River, Prentice Hall: 267.

OWEN D.R.J., FAWKES A.J., 1983. Engineering Fracture Mechanics, Numerical Methods and Application. Swansea, Pineridge Press Ltd.: 305.

SIH G.C., 1978. Mechanics of fracture – stress analysis of notch problems. Alphen aan den Rijn, Noordhoﬀ Interna-tional Publishing: 198.

SIH G.C., 1973. Handbook of Stress Intensity Factors. PA, Lehigh University.

SIH G.C., LIEBOWITZ H., 1968. Mathematical Theories of Brittle Fracture. In: LIEBOWITZ H. (ed.), Fracture, Vol. II. New York, London, Academic Press: 67–190.

Received for publication July 1, 2005 Accepted after corrections September 12, 2005

**Matematické funkce pro popis tranzitních křivek**

**ABSTRAKT: Jednou z důležitých vlastností materiálů je houževnatost. Nejpoužívanějším konstrukčním materiálem je **
v současné době stále ocel. Tento materiál se v závislosti na teplotě může porušit jak křehce, tak i houževnatě, a proto
hledáme teplotu, nad kterou se bude porušovat houževnatě. Jednou z metod, jak zjistit houževnatost teplotně-tranzitním
přístupem, je zkouška rázem v ohybu podle Charpyho v určitém teplotním intervalu. Soubor takto naměřených dat je velký
a vyžaduje proložení křivkou, která nám reprezentuje závislost nárazové práce na teplotě.

**Klíčová slova: tranzitní křivka; tranzitní teplota; nárazová práce**

*Corresponding author:*

Ing. ROSTISLAV CHOTĚBORSKÝ, Ph.D., Česká zemědělská univerzita v Praze, Technická fakulta, katedra materiálu a strojírenské technologie, 165 21 Praha 6-Suchdol, Česká republika